multiple useful applications. In the metallurgy industry, refractories are used for lining furnaces, kilns, reactors, and other vessels which hold and transport hot media such as metal and slag. Refractories have other high temperature applications such as fired heaters, hydrogen reformers, ammonia primary and secondary reformers, cracking furnaces, utility boilers, catalytic cracking units, air heaters, and sulfur furnaces. Classification of refractory materials Refractories are classified in multiple ways, based on: Chemical composition Method of manufacture Fusion temperature Refractoriness Thermal conductivity Based on chemical composition Acidic refractories Acidic refractories are generally impervious to acidic materials but easily attacked by basic materials, and are thus used with acidic slag in acidic environments. They include substances such as silica, alumina, and fire clay brick refractories. Notable reagents that can attack both alumina and silica are hydrofluoric acid, phosphoric acid, and fluorinated gases (e.g. HF, F2). At high temperatures, acidic refractories may also react with limes and basic oxides. Silica refractories are refractories containing more than 93% silicon oxide (SiO2). They are acidic, have high resistance to thermal shock, flux and slag resistance, and high spalling resistance. Silica bricks are often used in the iron and steel industry as furnace materials. An important property of silica brick is its ability to maintain hardness under high loads until its fusion point. Silica refractories are usually cheaper hence easily disposable. New technologies that provide higher strength and more casting duration with less silicon oxide (90%) when mixed with organic resins have been developed. Zirconia refractories are refractories primarily composed of zirconium oxide (ZrO2). They are often used for glass furnaces because they have low thermal conductivity, are not easily wetted by molten glass and have low reactivity with molten glass. These refractories are also useful for applications in high temperature construction materials. Aluminosilicate refractories mainly consist of alumina (Al2O3) and silica (SiO2). Aluminosilicate refractories can be semiacidic, fireclay composite, or high alumina content composite. Basic refractories Basic refractories are used in areas where slags and atmosphere are basic. They are stable to alkaline materials but can react to acids, which is important e. g. when removing phosphorus from pig iron (see Gilchrist–Thomas process). The main raw materials belong to the RO group, of which magnesia (MgO) is a common example. Other examples include dolomite and chrome-magnesia. For the first half of the twentieth century, the steel making process used artificial periclase (roasted magnesite) as a furnace